- Nano Express
- Open Access
In Situ-Formed and Low-Temperature-Deposited Nb:TiO2 Compact-Mesoporous Layer for Hysteresis-Less Perovskite Solar Cells with High Performance
Nanoscale Research Letters volume 15, Article number: 135 (2020)
Recently, reported perovskite solar cells (PSCs) with high power conversion efficiency (PCE) are mostly based on mesoporous structures containing mesoporous titanium oxide (TiO2) which is the main factor to reduce the overall hysteresis. However, existing fabrication approaches for mesoporous TiO2 generally require a high-temperature annealing process. Moreover, there is still a long way to go for improvement in terms of increasing the electron conductivity and reducing the carrier recombination. Herein, a facile one-step, in situ, and low-temperature method was developed to prepare an Nb:TiO2 compact-mesoporous layer which served as both scaffold and electron transport layer (ETL) for PSCs. The Nb:TiO2 compact-mesoporous ETL-based PSCs exhibit suppressed hysteresis, which is attributed to the synergistic effect of the increased interface surface area caused by nano-pin morphology and the improved carrier transportation caused by Nb doping. Such a high-quality compact-mesoporous layer allows the PSCs assembled using optimized 2% Nb-doped TiO2 to achieve a remarkable PCE of 19.74%. This work promises an effective approach for creating hysteresis-less and high-efficiency PSCs based on compact-mesoporous structures with lower energy consumption and cost.
Organic-inorganic hybrid perovskites have been attracting great interest as promising light-absorbing materials owing to their large absorption coefficients, high carrier mobility, and ease of fabrication [1,2,3,4,5]. Perovskite-based solar cells, photodetectors, light-emitting diodes (LEDs), and even memory devices have been widely investigated and established [6,7,8]. Since the year 2009, the power conversion efficiency of perovskite solar cells (PSCs) has maintained rapid growth from 3.8% to over 25% under standard AM 1.5 illumination [9,10,11,12]. PSCs are generally fabricated with a mesoporous or planar structure [13,14,15]. To date, the reported PSCs with high power conversion efficiency (PCE) are typically based on a mesoporous structure containing an indispensable scaffold layer of metal oxide . Titanium oxide (TiO2) has been commonly used as an electron transport layer. The typical mesoporous-type PSC presented by Seok has a structure of FTO/compact TiO2/mesoporous TiO2 and perovskite composite layer/perovskite upper layer/PTAA/Au . It is generally known that the mesoporous TiO2 contributes most to reduce the overall hysteresis for mesoporous-type PSCs . However, the fabrication of a mesoporous TiO2 layer often requires a high-temperature (> 450 °C) annealing treatment, leading to large energy consumption and limiting its application in flexible devices [19,20,21]. Compared with the mesoporous-type PSCs, planar-type PSCs can be fabricated using a low-temperature and low-cost process . However, planar-type PSCs usually suffer from poor electron conductivity, severe charge recombination, and relatively lower crystallinity, resulting in low PCE with severe hysteresis behavior [23, 24].
Extensive efforts have been made to develop high-quality TiO2 electron transport layers (ETLs) with high electron mobility, such as through morphology optimization, surface modifications, and doping. In particular, a wide range of elements have been chosen to prepare TiO2 doping layers in PSCs, including Lithium (Li) [25, 26], Niobium (Nb) [27, 28], Platinum (Pt) , Sodium (Na) , Neodymium (Nd) , and Aluminum (Al) . For instance, Liu et al. reported that the Li-doped TiO2 ETL was beneficial to the performance of the mesoporous-structure PSCs, especially for alleviating the hysteresis effect . Liao et al. reported that the Pt-doped TiO2 ETL could improve the charge carrier extraction and injection efficiency in n-i-p PSCs . Other ions such as Na, Nb, and transition metal ions [30, 31, 33,34,35] were used to modify surface or passivate defect of TiO2, contributing to reducing non-radiative recombination. Among these elements, Niobium metal (Nb) is a good candidate as a doping material for titanium oxide electron transport materials due to its similar radius with that of titanium. The results shown by Yin et al. demonstrated that Nb doping could make an improvement in both conductivity and mobility, simultaneously decrease the trap-state density of TiO2 ETLs for PSCs . Despite these progresses, a relatively high-temperature (150 °C) treatment was mandatory and large hysteresis was still observed in PSCs based on Nb-doped TiO2. As is well known, current density-voltage (J-V) hysteresis is a critical issue that occurs frequently, especially in planar-structure PSC devices. Severe hysteresis can lead to instability of PSCs and degradation of PCE. For this reason, it is highly desired to develop a hysteresis-less PSC utilizing a simple and low-temperature method.
Here, we propose a facile one-step, in situ, and low-temperature (70 °C) strategy to develop hysteresis-less PSCs which contain a single Nb:TiO2 compact-mesoporous layer serving as both scaffold and ETL. The Nb:TiO2 layer contains a compact TiO2 bottom with nano-pin morphology on the surface, which can be utilized as a scaffold. The hysteresis index decreased significantly from 24.39% for the PSC based on bare TiO2 to 3.19% for that based on 2% Nb:TiO2 layer due to the collaborative effect of the increased interface surface area caused by nano-pin morphology on the surface and the improved carrier transportation rate because of the presence of Nb. The high-quality mesoporous layer allowed the PSCs to achieve remarkable PCE of 19.7%. This work promises an effective approach for achieving hysteresis-less and high-efficiency PSCs through scalable and inexpensive methods at low temperature.
First, the FTO substrates were successively put into acetone, alcohol, and deionized water to be ultrasonic cleaned of 30 min each. After that, the cleaned substrates were treated by a UV-ozone cleaner for 20 min and then placed in a petri dish. Second, liquid TiCl4 was dropped into deionized water under the temperature of 0 °C to prepare 0.1 M TiCl4 aqueous solution. Third, NbCl5 powder was put into the ethanol near the temperature of 0 °C to obtain 0.1 M NbCl5 ethanol solution. Then, X vol.% NbCl5 ethanol solution and (100-X) vol.% TiCl4 aqueous solution were dropped onto the surface of FTO substrates sequentially inside the petri dish. After hydrothermal reacting at 70 °C for 60 min, the Nb:TiO2 nano-pin feature was formed on the FTO substrates.
The perovskite absorption layer was deposited with the dynamic two-step spin-coating method . First, the PbI2 precursor solution was obtained by adding 0.462 g PbI2 into 1 mL DMF. Meanwhile, the CH3NH3I (MAI) precursor solution was obtained by adding 0.1 g MAI into 2 mL isopropanol (99.5%, Aladdin). Second, 55 μL PbI2 precursor solution was spun onto the as-prepared Nb:TiO2 ETL film at 3000 rpm for 10 s. At this moment, 55 μL MAI precursor solution was dropped onto the sample immediately, and spinning was continued for 20 s. Finally, the whole film was annealed at 150 °C for 15 min.
The HTL precursor was obtained by stirring 1 mL chlorobenzene solution, which contained 72.3 mg Spiro-OMeTAD, 28 μL 4-tert-butylpyridine, and 17 μL Li-TFSI solution (520 mg mL−1). The precursor was spin-coated onto perovskite film at 2000 rpm for 30 s. Then, the Spiro-OMeTAD HTL with a thickness of around 250 nm was obtained.
A field-emission scanning electron microscope (FE-SEM, SU8010, Hitachi) was carried out to study the morphologies of the samples. The absorption spectra were recorded with a UV-vis spectrophotometer (Shimadzu, UV-3600). Electrochemical impedance spectroscopy (EIS) was employed to understand the carrier transportation process by an electrochemical workstation (Autolab, PGSTAT 302 N). The current density-voltage (J-V) measurement was recorded using a digital source (Keithley 2400) with the assistance of the solar simulator (ABET Technologies, SUN 3000).
Results and Discussion
A schematic of the PSC structure and the Nb:TiO2 synthesis procedure is shown in Fig. 1. First, the cleaned FTO substrates were faced up placed in a petri dish. Second, 1 mL NbCl5 ethanol solution and 49 mL TiCl4 aqueous solution were poured onto the FTO substrates in the dish sequentially. Third, the dish was transferred into an oven and hydrothermal reacted at 70 °C for 1 h. Finally, the TiO2 layer with nano-pin morphology and 2% Nb doping ratio was formed on the FTO substrates. For the preparation of the control TiO2 layer, only TiCl4 aqueous solution (without NbCl5 ethanol solution) was dropped into the dish containing FTO substrates.
To understand the effect of Nb doping on the evolution of the TiO2 layer, the morphologies of the control TiO2 and Nb-doped TiO2 were investigated using scanning electron microscopy (SEM) which is shown in Fig. 2. The bare TiO2 exhibits a much smoother surface, which is a typical morphology of compact TiO2 layers in planar PSCs. However, 2% Nb-doped TiO2 shows a nano-pin texture distributed on the compact bottom. The length of the nano-pin was determined to be 50 ± 20 nm. This indicates that the Nb:TiO2 layer contains a compact TiO2 layer with a nano-pin morphology on the surface, which is regarded as a mesoporous layer. Therefore, this in situ formed Nb:TiO2 compact-mesoporous layer, which was obtained by a one-step process, actually serves as both a scaffold and an ETL in the PSC. The formation of nano-pin morphology resulted from the hydrothermal reacting with the assistance of NbCl5 ethanol solution.
The XPS spectra of 2% Nb:TiO2 film is shown in Fig. 3. Figure 3a shows the full scan spectra of the 2% Nb:TiO2 film. It is found that the atom ratio of Nb/Ti (1.3%) is closed to the element doping ratio of 2% in the precursor mixture. As shown in Fig. 3b, the Gaussian peaks located at 458 eV and 464 eV are corresponding to the binding energy of Ti 2p3/2 and Ti 2p1/2. Similarly, the Gaussian fitted lines of Nb5+ can be deconvolved into two individual peaks which are associated with Nb 3d5/2 and Nb 3d3/2, respectively, at the binding energy of 207 eV and 209 eV (Fig. 3c). The XPS spectra demonstrate the successful doping of Nb in the TiO2 film.
Figure 4a shows the absorption spectra of FTO, bare TiO2/FTO, and Nb-doped TiO2/FTO. Both bare TiO2 and Nb-doped TiO2 exhibit main absorption edge at the wavelength of 300–350 nm. The absorption curve of Nb-doped TiO2 almost overlaps that of bare TiO2. The energy bandgap (Eg) can be calculated based on the absorption spectra using the Tauc equation, which is shown in Fig. 4b. The Eg is 4.05 eV for FTO and 3.5 eV for both bare TiO2 and Nb-doped TiO2. Therefore, it can be concluded that Nb doping has little influence on the absorption of TiO2. The transmittance is also not shifted during the Nb doping process as shown in Fig. S1.
Fig. S2 presents the SEM images of CH3NH3PbI3 perovskite films spin-coated on the bare TiO2 and Nb-doped TiO2 films. It is indicated that the perovskite films exhibit fewer pinholes and full surface coverage. Thanks to our previously developed non-substrate-selective dynamic two-step spin-coating strategy , the film uniformity and coverage can be better controlled. Besides, the average crystalline grain sizes of the perovskite films are very similar. Fig. S3 presents the absorption spectra of the perovskite films deposited on the bare TiO2 and Nb-doped TiO2 films. No obvious difference in absorption peak is observed between the perovskite films. These results suggest that the nano-pin morphology formation on the Nb-doped TiO2 compact-mesoporous layer could have little effect on the perovskite crystallization by dynamic two-step spin-coating strategy.
To understand the carrier transportation crossing the ETL/perovskite interfaces, the electrical impedance spectroscopy (EIS) was employed. PSCs were fabricated with the structure of FTO/TiO2/perovskite film/Spiro-OMeTAD/Au. Figure 5 shows the Nyquist plots of PSCs based on bare TiO2 and 2% Nb:TiO2 layers, and the corresponding equivalent circuit model is shown in the inset. The parameters of EIS were listed in Supplementary Table S1. It is known that the EIS contains two circular arcs . The high-frequency component is attributed to the charge transport resistance (Rct), and the low-frequency component is mainly related to the recombination resistance (Rrec) . In this comparison, everything but the perovskite/ETL interface was identical. Thus, only the Nb doping process should be responsible for the resistance (Rct and Rrec) variation. Compared to the bare TiO2 device, the Nb:TiO2 device exhibits smaller Rct and larger Rrec. The small Rct contributes to more efficient electron extraction, and the large Rrec proves lower charge recombination. These results confirm that the Nb:TiO2-based compact-mesoporous layer is an effective ETL for both charge transportation improving and carrier recombination rate reducing.
As shown in Fig. 6, the dependence of the PCE of PSCs on the Nb doping contents was investigated. The detail parameters for PSCs with different Nb doping concentrations varying from 0 to 8% was shown in Table 1. It is found that the doping ratio affects the open-circuit voltage (Voc) and fill factor (FF), which were first increased and then decreased with increasing Nb doping. The device with a 2% Nb-doped TiO2 layer exhibits the highest Voc of 1.19 eV, Jsc of 23.52 mA/cm2, and FF of 70.74%, leading to a PCE as high as 19.74% for the champion devices. Thanks to better carrier transportation, all parameters show notable improvement. However, superfluous doping would strengthen the carrier scattering and lead to poor mobility. The incremental recombination will weaken the carrier transport improvement and eventually harm the PCE.
The measured J-V curves of the control and champion device are shown in Fig. 7. It is well known that J-V hysteresis behavior often occurs, especially in planar-structure PSC devices. In this work, the hysteresis of J-V curves of bare compact TiO2-based PSC and 2% Nb:TiO2 compact-mesoporous layer-based PSC were examined. The hysteresis index, (PCE of reverse scan − PCE of forward scan)/PCE of reverse scan , reduced markedly from 24.39% for the PSC based on bare compact TiO2 to 3.19% for the PSC based on 2% Nb-doped TiO2 layer. It is well known that PSCs based on a mesoporous TiO2 layer can collect electrons and effectively achieve a balance between the hole flux and electron flux due to its larger surface area, thereby exhibiting less hysteresis . The hysteresis suppression of the Nb-doped TiO2-based device is motivated by the conductance increasing and the nano-pin morphology forming. Charge accumulation caused by interfacial capacitance at the ETL/perovskite interface would be reduced and result in hysteresis-less character.
We have developed a facile one-step, in situ, and low-temperature approach to achieve an Nb:TiO2 compact-mesoporous layer that serves as both scaffold and ETL for PSCs. As a result, PSCs based on 2% Nb-doped TiO2 can exhibit a remarkable PCE of 19.74%, which is dramatically higher than that of the controlled TiO2-based device. The Nb:TiO2 layer contains a compact TiO2 bottom with nano-pin morphology on the surface, which can be utilized as a mesoporous layer. Due to the collaborative effect of a large interface surface area and improved carrier transportation rate, the hysteresis of the J-V curve is markedly reduced, with the hysteresis index decreasing significantly from 24.39 to 3.19%. This work promises an effective approach for achieving hysteresis-less and high-efficiency PSCs through a well-designed scalable and cost-efficiency hydrothermal method at low temperature.
Availability of Data and Materials
The authors declare that the materials and data are available to the readers, and all conclusions made in this manuscript are based on the data which are all presented and shown in this paper.
Perovskite solar cells
Power conversion efficiency
- TiO2 :
Electron transport layer
Scanning electron microscope
Electrochemical impedance spectroscopy
- B g :
- E g :
- V oc :
- J sc :
Short circuit current density
Yang M, Li Z, Reese M et al (2017) Perovskite ink with wide processing window for scalable high-efficiency solar cells. Nat Energy 2(5):17038–17047
Zhao D, Chen C, Wang C et al (2018) Efficient two-terminal all-perovskite tandem solar cells enabled by high-quality low-bandgap absorber layers. Nat Energy 3(12):1093–1100
Shi D, Adinolfi V, Comin R et al (2015) Low trap-state density and long carrier diffusion in organolead trihalide perovskite single crystals. Science 347(6221):519–522
Sun H, Lei T, Tian W et al (2017) Self-powered, flexible, and solution-processable perovskite photodetector based on low-cost carbon cloth. Small 13(28):1701042–1701049
Sun H, Tian W, Cao F et al (2018) Ultrahigh-performance self-powered flexible double-twisted fibrous broadband perovskite photodetector. Adv Mater 30(21):1706986–1706993
Zhao Y, Li C, Shen L (2019) Recent advances on organic-inorganic hybrid perovskite photodetectors with fast response. InfoMat 1(2):164–182
Zhao X, Xu H, Wang Z et al (2019) Memristors with organic-inorganic halide perovskites. InfoMat 1(2):183–210
Fang T, Zhang F, Yuan S et al (2019) Recent advances and prospects toward blue perovskite materials and light-emitting diodes. InfoMat 1(2):211–233
National renewable energy laboratory. Best research-cell efficiency chart. https://www.nrel.gov/pv/cell-efficiency.html. Accessed 6 Apr 2020.
Zhang F, Zhu K (2019) Additive engineering for efficient and stable perovskite solar cells. Adv Energy Mater 10(13):1902579–19025605
Lu P, Lu M, Wang H et al (2019) Metal halide perovskite nanocrystals and their applications in optoelectronic devices. InfoMat 1(4):430–459
Luo J, Xia J, Yang H et al (2020) Novel approach toward hole-transporting layer doped by hydrophobic Lewis acid through infiltrated diffusion doping for perovskite solar cells. Nano Energy 70:104509–104519
Lee M, Teuscher J, Miyasaka T et al (2012) Efficient hybrid solar cells based on meso-superstructured organometal halide perovskites. Science 338(6107):643–647
Fakharuddin A, Schmidt-Mende L, Garcia-Belmonte G et al (2017) Interfaces in perovskite solar cells. Adv Energy Mater 7(22):1700623
Sun H, Zhou Y, Xin Y et al (2019) Composition and energy band-modified commercial FTO substrate for in situ formed highly efficient electron transport layer in planar perovskite aolar cells. Adv Funct Mater 29(11):1808667–1808676
Yang D, Yang R, Wang K et al (2018) High efficiency planar-type perovskite solar cells with negligible hysteresis using EDTA-complexed SnO2. Nat Commun 9(1):1–11
Yang W, Park B, Jung E et al (2017) Iodide management in formamidinium-lead-halide-based perovskite layers for efficient solar cells. Science 356(6345):1376–1379
Ravishankar S, Gharibzadeh S, Roldán-Carmona C et al (2018) Influence of charge transport layers on open-circuit voltage and hysteresis in perovskite solar cells. Joule 2(4):788–798
Hao D, Zou J, Huang J (2020) Recent developments in flexible photodetectors based on metal halide perovskite. InfoMat 2(1):139–169
Yella A, Heiniger L, Gao P et al (2014) Nanocrystalline rutile electron extraction layer enables low-temperature solution processed perovskite photovoltaics with 13.7% efficiency. Nano Lett 14(5):2591–2596
Mabrouk S, Bahrami B, Elbohy H et al (2019) Synergistic engineering of hole transport materials in perovskite solar cells. InfoMat. https://doi.org/10.1002/inf2.12062
Cai F, Yang L, Yan Y et al (2017) Eliminated hysteresis and stabilized power output over 20% in planar heterojunction perovskite solar cells by compositional and surface modifications to the low-temperature-processed TiO2 layer. J Mater Chem A 5(19):9402–9411
Ren X, Liu Y, Lee D et al (2020) Chlorine-modified SnO2 electron transport layer for high-efficiency perovskite solar cells. InfoMat 2(2):401–408
Jiang J, Jin Z, Lei J et al (2017) ITIC surface modification to achieve synergistic electron transport layer enhancement for planar-type perovskite solar cells with efficiency exceeding 20%. J Mater Chem A 5:9514–9522
Giordano F, Abate A, Correa B et al (2016) Enhanced electronic properties in mesoporous TiO2 via lithium doping for high-efficiency perovskite solar cells. Nat Commun 7:10379–10385
Liu D, Li S, Zhang P et al (2017) Efficient planar heterojunction perovskite solar cells with Li-doped compact TiO2 layer. Nano Energy 31:462–468
Yin G, Ma J, Jiang H et al (2017) Enhancing efficiency and stability of perovskite solar cells through Nb-doping of TiO2 at low temperature. ACS Appl Mater Interfaces 9(12):10752–10758
Chen B, Rao H, Li W et al (2016) Achieving high-performance planar perovskite solar cell with Nb-doped TiO2 compact layer by enhanced electron injection and efficient charge extraction. J Mater Chem A 4(15):5647–5653
Jiang L, Wang Z, Li M et al (2018) Enhanced electrical property of compact TiO2 layer via platinum doping for high-performance perovskite solar cells. Sol RRL 2(11):1800149–1800157
Hou Y, Scheiner S, Tang X et al (2017) Suppression of hysteresis effects in organohalide perovskite solar cells. Adv Mater Interfaces 4(11):1700007–1700016
Roose B, Godel K, Pathak S et al (2016) Enhanced efficiency and stability of perovskite solar cells through Nd-doping of mesostructured TiO2. Adv Energy Mater 6(2):1501868–1501875
Pathak S, Abate A, Ruckdeschel P et al (2014) Performance and stability enhancement of dye-sensitized and perovskite solar cells by Al doping of TiO2. Adv Funct Mater 24(38):6046–6055
Liang C, Li P, Zhang Y et al (2017) Mild solution-processed metal-doped TiO2 compact layers for hysteresis-less and performance-enhanced perovskite solar cells. J Power Sources 372:235–244
Song J, Li S, Zhao Y et al (2017) Performance enhancement of perovskite solar cells by doping TiO2 blocking layer with group VB elements. J Alloys Compd 694:1232–1238
Kang D, Park N (2019) On the current-voltage hysteresis in perovskite solar cells: dependence on perovskite composition and methods to remove hysteresis. Adv Mater 31(34):1805214
Sun H, Deng K, Zhu Y et al (2018) A novel conductive mesoporous layer with a dynamic two-step deposition strategy boosts efficiency of perovskite solar cells to 20%. Adv Mater 30(28):1801935–1801943
Zhang Z, Li J, Wang X et al (2017) Enhancement of perovskite solar cells efficiency using N-Doped TiO2 nanorod arrays as electron transfer layer. Nanoscale Res Lett 12(1):43–50
Liu D, Yang J, Kelly T (2014) Compact layer free perovskite solar cells with 13.5% efficiency. J Am Chem Soc 136(49):17116–17122
I would like to express my gratitude to the financial support from the National Natural Science Foundation of China (51972042) and the Fundamental Research Funds for the Central Universities (Y0301902300100112).
This research was supported by the National Natural Science Foundation of China (51972042) and the Fundamental Research Funds for the Central Universities (Y0301902300100112).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
The light permeation comparison of TiO2 and Nb:TiO2 based ETL. Figure S2. SEM images of (a) perovskite deposited on the pure TiO2 and (b) perovskite deposited on the TiO2 layer doped with 2% Nb. Figure S3. Absorbance spectra of perovskite film deposited on pure TiO2 and 2%Nb:TiO2 layer. Table S1. Parameters employed for the fitting of the impedance spectra of devices based on the pure TiO2 and 2% Nb:TiO2
About this article
Cite this article
Yu, M., Sun, H., Huang, X. et al. In Situ-Formed and Low-Temperature-Deposited Nb:TiO2 Compact-Mesoporous Layer for Hysteresis-Less Perovskite Solar Cells with High Performance. Nanoscale Res Lett 15, 135 (2020). https://doi.org/10.1186/s11671-020-03366-1
- Perovskite solar cells
- Titanium oxide